Description

Design and global optimization of high-efficiency thermophotovoltaic systems

All materials on our website are shared by users. If you have any questions about copyright issues, please report us to resolve them. We are always happy to assist you.

Related Documents

Share

Transcript

Design and global optimization of high-efﬁciency thermophotovoltaicsystems
Peter Bermel
1
,
2
,
3
,
4
∗
, Michael Ghebrebrhan
2
,
4
, Walker Chan
3
, Yi XiangYeng
1
,
3
, Mohammad Araghchini
1
, Raﬁf Hamam
2
,
4
, Christopher H.Marton
3
,
5
, Klavs F. Jensen
3
,
5
, Marin Solja ˇci´c
1
,
2
,
3
,
4
, John D.Joannopoulos
1
,
2
,
3
,
4
, Steven G. Johnson
1
,
6
, Ivan Celanovic
3
1
Research Laboratory of Electronics, Massachusetts Institute of Technology, 77 Massachusetts Ave., Cambridge, MA 02139, USA
2
Department of Physics, Massachusetts Institute of Technology, 77 Massachusetts Ave.,Cambridge, MA 02139, USA
3
Institute for Soldier Nanotechnologies, Massachusetts Institute of Technology, 77 Massachusetts Ave., Cambridge, MA 02139, USA
4
Center for Materials Science and Engineering, Massachusetts Institute of Technology, 77 Massachusetts Ave., Cambridge, MA 02139, USA
5
Department of Chemical Engineering, Massachusetts Institute of Technology, 77 Massachusetts Ave., Cambridge, MA 02139, USA
6
Department of Mathematics, Massachusetts Institute of Technology, 77 Massachusetts Ave.,Cambridge, MA 02139, USAbermel@mit.edu
Abstract:
Despite their great promise, small experimental thermophotovoltaic (TPV)systems at 1000 K generally exhibit extremely low power conversion efﬁ-ciencies (approximately 1%), due to heat losses such as thermal emissionof undesirable mid-wavelength infrared radiation. Photonic crystals (PhC)have the potential to strongly suppress such losses. However, PhC-baseddesigns present a set of non-convex optimization problems requiringefﬁcient objective function evaluation and global optimization algorithms.Both are applied to two example systems: improved micro-TPV generatorsand solar thermal TPV systems. Micro-TPV reactors experience up to a27-fold increase in their efﬁciency and power output; solar thermal TPVsystems see an even greater 45-fold increase in their efﬁciency (exceedingthe Shockley–Quiesser limit for a single-junction photovoltaic cell).
© 2010 Optical Society of America
OCIS codes:
(230.5298) Photonic crystals; (350.6050) Solar energy.
References and links
1. H. H. Kolm, “Solar-battery power source,” Tech. rep., MIT Lincoln Laboratory (1956). Quarterly Progress Re-port, Group 35, p. 13.2. B. Wedlock, “Thermo-photo-voltaic conversion,” Proc. IEEE
51
, 694–698 (1963).3. R. Black, P. Baldasaro, and G. Charache, “Thermophotovoltaics - development status and parametric considera-tions for power applications,” in
International Conference on Thermoelectrics
, 18, pp. 639–644 (1999).4. F. O’Sullivan, I. Celanovic, N. Jovanovic, J. Kassakian, S. Akiyama, and K. Wada, “Optical characteristics of 1DSi/SiO2 photonic crystals for thermophotovoltaic applications,” J. Appl. Phys.
97
, 033,529 (2005).
5. H. Xue, W. Yang, S. Chou, C. Shu, and Z. Li, “Microthermophotovoltaics power system for portable MEMSdevices,” Nanoscale Microscale Thermophys. Eng.
9
, 85–97 (2005).6. J. D. Joannopoulos, S. G. Johnson, J. N. Winn, and R. D. Meade,
Photonic Crystals: Molding the Flow of Light
,2nd ed. (Princeton, Princeton, NJ, 2008).7. A. Heinzel, V. Boerner, A. Gombert, B. Blasi, V. Wittwer, and J. Luther, “Radiation ﬁlters and emitters for theNIR based on periodically structured metal surfaces,” J. Mod. Opt.
47
(2000).8. J. M. Gee, J. B. Moreno, S.-Y. Lin, and J. G. Fleming, “Selective emitters using photonic crystals for thermopho-tovoltaic energy conversion,” in
Twenty-ninth IEEE Photovolt. Spec. Conf.
(2002).9. H. Sai, Y. Kanamori, and H. Yugami, “High-temperature resistive surface grating for spectral control of thermalradiation,” Appl. Phys. Lett.
82
, 1685–1687 (2003).10. U. Ortabasi and B. Bovard, “Rugate technology for thermophotovoltaic applications: a new approach to nearperfect ﬁlter performance,” AIP Conf. Proc.
653
, 249–258 (2003).11. I. Celanovic, D. Perreault, and J. Kassakian, “Resonant-cavity enhanced thermal emission,” Phys. Rev. B
72
,075,127 (2005).12. D. L. Chan, I. Celanovic, J. D. Joannopoulos, and M. Soljacic, “Emulating one-dimensional resonant
Q
-matchingbehavior in a two-dimensional system via Fano resonances,” Phys. Rev. A
74
, 064,901 (2006).13. I. Celanovic, N. Jovanovic, and J. Kassakian, “Two-dimensional tungsten photonic crystals as selective thermalemitters,” Appl. Phys. Lett.
92
, 193,101–193,103 (2008).14. T. D. Rahmlow, D. M. DePoy, P. M. Fourspring, H. Ehsani, J. E. Lazo-Wasem, and E. J. Gratrix, “Development of frontsurface,spectralcontrolﬁlterswithgreatertemperaturestabilityforthermophotovoltaicenergyconversion,”AIP Conf. Proc.
890
, 59–67 (2007).15. S. John and R. Wang, “Metallic photonic band-gap ﬁlament architectures for optimized incandescent lighting,”Phys. Rev. A
78
, 043,809 (2008).16. J. Gee, “Optically enhanced absorption in thin silicon layers using photonic crystals,” in
Twenty-Ninth IEEE Photovolt. Spec. Conf.
, pp. 150–153 (2002).17. M. Ghebrebrhan, P. Bermel, Y. Avniel, J. D. Joannopoulos, and S. G. Johnson, “Global optimization of siliconphotovoltaic cell front coatings,” Opt. Express
17
, 7505–7518 (2009).18. B. Chachuat, A. Mitsos, and P. I. Barton, “Optimal design and steady-state operation of micro power generationemploying fuel cells,” Chem. Eng. Sci.
60
(2005).19. M. Yunt, B. Chachuat, A. Mitsos, and P. I. Barton, “Designing man-portable power generation systems for vary-ing power demand,” Process Syst. Eng.
54
, 1254 (2008).20. L. Li, “Formulation and comparison of two recursive matrix algorithms for modeling layered diffraction grat-ings,” J. Opt. Soc. Am. A
13
, 1024–1035 (1996).21. D. Whittaker and I. Culshaw, “Scattering-matrix treatment of patterned multilayer photonic structures,” Phys.Rev. B
60
, 2610–2618 (1999).22. P. Bienstman, “Rigorous and efﬁcient modelling of wavelength scale photonic components,” Ph.D. thesis, Uni-versity of Ghent, Belgium (2001).23. A. Taﬂove and S. C. Hagness,
Computational Electrodynamics
, 2nd ed. (Artech House, Norwood, MA, 2000).24. A. F. Oskooi, D. Roundy, M. Ibanescu, P. Bermel, J. D. Joannopoulos, and S. G. Johnson, “MEEP: A ﬂexiblefree-software package for electromagnetic simulations by the FDTD method,” Comp. Phys. Comm.
181
, 687–702 (2010).25. C. Herzinger, B. Johs, W. McGahan, J. Woollam, and W. Paulson, “Ellipsometric determination of optical con-stants for silicon and thermally grown silicon dioxide via a multi-sample, multi-wavelength, multi-angle investi-gation,” J. Appl. Phys.
83
, 3323–3336 (1998).26. J. Zhao and M. Green, “Optimized Antireﬂection Coatings for High-Efﬁciency Silicon Solar Cells,” IEEE Trans.Electron Dev.
38
, 1925 (1991).27. G. Rybicki and A. Lightman,
Radiative processes in astrophysics
(John Wiley and Sons, 1979).28. S. Kucherenko and Y. Sytsko, “Application of deterministic low-discrepancy sequences in global optimization,”Computational Optimization and Applications
30
, 297–318 (2005).29. M. Powell,
Advances in Optimization and Numerical Analysis
(Kluwer Academic, Dordrecht, Holland, 1994).30. J. M. Gablonsky and C. T. Kelley, “A locally-biased form of the DIRECT algorithm,” J. Global Optim.
21
(1),27–37 (2001).31. R. C. Pilawa-Podgurski, N. A. Pallo, W. R. Chan, D. J. Perreault, and I. L. Celanovic, “Low-power maximumpower point tracker with digital control for thermophotovoltaic generators,” 25th IEEE Applied Power Electron-ics Conference, 961–967 (2010).32. C. Miesse, R. Masel, C. Jensen, M. Shannon, and M. Short, “Submillimeter-scale combustion,” AIChE J.
50
,3206–3214 (2004).33. S. Deshmukh and D. Vlachos, “A reduced mechanism for methane and one-step rate expressions for fuel-leancatalytic combustion of small alkanes on noble metals,” Combust. Flame
149
, 366–383 (2007).34. B. Blackwell, “Design, fabrication, and characterization of a micro fuel processor,” Ph.D. thesis, MassachusettsInstitute of Technology (2008).35. C. A. Wang, H. Choi, S. Ransom, G. Charache, L. Danielson, and D. DePoy, “High-quantum-efﬁciency 0.5 eV
GaInAsSb/GaSb thermophotovoltaic devices,” Appl. Phys. Lett.
75
, 1305–1307 (1999).36. M. W. Dashiell, J. F. Beausang, H. Ehsani, G. Nichols, D. M. DePoy, L. R. Danielson, P. Talamo, K. D. Rahner,E. J. Brown, S. R. Burger, P. M. Fourspring, W. F. T. Jr., P. Baldasaro, C. A. Wang, R. K. Huang, M. K. Connors,G. W. Turner, Z. A. Shellenbarger, G. Taylor, J. Li, R. Martinelli, D. Donetski, S. Anikeev, G. L. Belenky, andS. Luryi, “Quaternary InGaAsSb thermophotovoltaic diodes,” IEEE Trans. Electron Dev.
53
, 2879–2891 (2006).37. S. Sze,
Physics of Semiconductor Devices
(Wiley and Sons, New York, 1981).38. W. Chan, R. Huang, C. A. Wang, J. Kassakian, J. D. Joannopoulos, and I. Celanovic, “Modeling low-bandgapthermophotovoltaic diodes for high-efﬁciency portable power generators,” Sol. Energy Mater. Sol. Cells
94
, 509–514 (2010).39. P. Wilkinson, “Photonic Bloch oscillations and Wannier-Stark ladders in exponentially chirped Bragg gratings,”Phys. Rev. E
65
, 056,616 (2002).40. C. Henry, “Limiting efﬁciencies of ideal single and multiple energy gap terrestrial solar cells,” J. Appl. Phys.
51
,4494–4500 (1980).41. B. G. Bovard, “Rugate ﬁlter theory: an overview,” Appl. Opt.
32
, 5427–5442 (1993).42. J.-Q. Xi, M. F. Schubert, J. K. Kim, E. F. Schubert, M. Chen, S.-Y. Lin, W. Liu, and J. A. Smart, “Optical thin-ﬁlm materials with low refractive index for broadband elimination of Fresnel reﬂection,” Nature Photonics
1
,176–179 (2007).43. A. Yariv, Y. Xu, R. K. Lee, and A. Scherer, “Coupled-resonator optical waveguide: a proposal and analysis,” Opt.Lett.
24
, 711–713 (1999).44. M. Ghebrebrhan, P. Bermel, Y. X. Yeng, J. D. Joannopoulos, M. Soljacic, and I. Celanovic, “Tailoring thermalemission via
Q
-matching of photonic crystal resonances,” (2010). To be submitted, Phys. Rev. A.45. W. Spirkl and H. Ries, “Solar thermophotovoltaics: an assessment,” J. Appl. Phys.
57
, 4409–4414 (1985).46. N. Harder and P. Wurfel, “Theoretical limits of thermophotovoltaic solar energy conversion,” Semicond. Sci.Technol.
18
, S151 (2003).47. A. Luque, “Solar Thermophotovoltaics: Combining Solar Thermal and Photovoltaics,” AIP Conf. Proc.
890
,3–16 (2007).48. A. Datas, C. Algora, V. Corregidor, D. Martin, A. Bett, F. Dimroth, and J. Fernandez, “Optimization of Germa-nium Cell Arrays in Tungsten Emitter-based Solar TPV Systems,” AIP Conf. Proc.
890
, 227–237 (2007).49. E. Rephaeli and S. Fan, “Absorber and emitter for solar thermophotovoltaic systems to achieve efﬁciency ex-ceeding the Shockley-Queisser limit,” Opt. Express
17
, 15,145–15,159 (2009).50. ASTMG173-03,
Standard Tables for Reference Solar Spectral Irradiances: Direct Normal and Hemisphericalon 37 degree Tilted Surface
(ASTM International, West Conshohocken, Pennsylvania, 2005).51. T. Sathiaraj, R. Thangarj, A. Sharbaty, M. Bhatnagar, and O. Agnihotri, “Ni-Al
2
O
3
selective cermet coatings forphotochemical conversion up to 500
◦
C,” Thin Solid Films
190
, 241 (1990).52. Q.-C. Zhang, “High efﬁciency Al-N cermet solar coatings with double cermet layer ﬁlm structures,” J. Phys. D:Appl. Phys.
32
, 1938–1944 (1999).53. C. Kennedy, “Review of mid- to high-temperature solar selective absorber materials,” Tech. Rep. TP-520-31267,National Renewable Energy Laboratory (2002).54. N. Sergeant, O. Pincon, M. Agrawal, and P. Peumans, “Design of wide-angle solar-selective absorbers usingaperiodic metal-dielectric stacks,” Opt. Express
17
, 22,800–22,812 (2009).55. N. Sergeant, M. Agrawal, and P. Peumans, “High performance solar-selective absorbers using sub-wavelengthgratings,” Opt. Express
18
, 5525–5540 (2010).56. Y. Varshni, “Temperature dependence of the energy gap in semiconductors,” Physica
34
, 149–154 (1967).57. C. Grein and S. John, “Polaronic band tails in disordered solids: combined effects of static randomness andelectron-phonon interactions,” Phys. Rev. B
39
, 1140 (1989).
1. Introduction
Thermophotovoltaic (TPV)systemsconvertheatintoelectricitybythermallyradiatingphotons,which are subsequently converted into electron-hole pairs via a low-bandgap photovoltaic (PV)medium; these electron-hole pairs are then conducted to the leads to produce a current [1–4].As solid-state devices, they have the potential for higher reliability, vastly smaller form fac-tors (meso- and micro-scales), and higher energy densities than traditional mechanical engines.However, most systems emit the vast majority of thermal photons with energies below the elec-tronic bandgap of the TPV cell, and are instead absorbed as waste heat. This phenomenon tendsto reduce TPV system efﬁciencies well below those of their mechanical counterparts operatingat similar temperatures, as shown in Fig. 1(a) [5]. Photon recycling via reﬂection of low-energyphotons with a 1D reﬂector is a concept that signiﬁcantly reduces radiative heat transfer [3,4].This approach can also be extended to encompass the more general concept of spectral shap-
Fig. 1. Approaches to TPV conversion of heat to electricity. The traditional design is de-picted in (a), and a novel approach based on manipulation of the photonic density of statesis depicted in (b). The anticipated increase in efﬁciency associated with the latter approachcan exceed 100%.
ing:directlysuppressingemissionofundesirable(belowbandgap)photonsaswellasenhancingemission of desirable (above bandgap) photons. Such control is provided by complex 1D, 2D,and 3D periodic dielectric structures, generally known as photonic crystals (PhCs) [6]. Spectralshaping has been proposed and predicted to be an effective approach for high-efﬁciency TPVpower generation [7–15]. This approach is illustrated in Fig. 1(b).Two speciﬁc classes of designs have already been studied in depth: narrow-band thermalemitters exhibiting wavelength, directional, and polarization selectivity [11,12], and wide-bandthermal emitters with emissivity close to that of a blackbody within the design range but muchlower outside the design range [7,9,13,15,16]. Intermediate-band designs combining featuresof each are also possible.However, the potential beneﬁts of exploring many designs can be overwhelmed by the difﬁ-culty of ﬁnding the optimum, as deﬁned by an appropriate ﬁgure of merit. In particular, the gen-eralized class of realistic multidimensional PhC design problems typically pose a non-convexoptimization problem, in which many local optima can exist [17]. Furthermore, power genera-tion in related systems, such as portable fuel cell devices, has also been demonstrated to posea non-convex optimization problem as well [18,19]. The problem at hand can be addressedvia carefully designed global optimization algorithms capable of navigating this complex land-scape.Inthispaper,twoexampleTPVsystemsofgreatrelevancearechosenandthenoptimized(with constraints): micro-TPV (
µ
TPV) generators and solar thermal TPV systems. It is shownthat appropriately chosen ﬁgures of merit can be increased by over an order of magnitude inboth cases, illustrating the tremendous promise of this approach.The remainder of this manuscript is structured as follows: in section 2, we discuss our com-
putational approach to simulating the performance of a single TPV design, as well as globallyoptimizing performance for entire TPV design classes. In section 3, we apply this technique tothe
µ
TPVgenerator, which usesahydrocarbon fuelmicro-combustor toheatour selective emit-ter. In section 4, we apply our computational approach to the solar thermal TPV system, whichposes the additional problem of optimizing a selective absorber for sunlight. We conclude bysummarizing our ﬁndings in section 5.
2. Computational Approach
The performance of the structures discussed in this paper are studied via a combination of op-tical and thermal models. Two tools are used to compute their absorptivity spectra. For layered1D and 2D structures, we use the transfer matrix method [20,21] implemented by a freely avail-able software package developed at the University of Ghent called CAMFR [22]. Plane waveradiation is applied from air at normal incidence, and ﬁelds are propagated through each layerto yield reﬂectance, transmittance, and absorptivity. Note that although in principle radiationshould be integrated over all angles, normal incidence is an excellent approximation for ourstructures up to angles of
±
π
/
3: see Fig. 12. For more complex 3D structures, we employ aﬁnite difference time-domain (FDTD) simulation [23] implemented via a freely available soft-ware package developed at MIT, known as Meep [24]. Again, a plane wave is sent from thenormal direction and propagated through space. On each grid point of a ﬂux plane deﬁnedat the front and back of the computational cell, the electric and magnetic ﬁelds are Fourier-transformed via integration with respect to preset frequencies at each time-step. At the end of the simulation, the Poynting vector is calculated for each frequency and integrated across eachplane, which yields the total transmitted and reﬂected power (ﬁrst subtracting the incident-ﬁeldFourier transforms for the latter) at each frequency [24]. To capture material dispersion, thec-Si regions are modeled with a complex dielectric constant that depends on wavelength, asin Ref. 25. The lower-index dielectric materials considered in this work generally have verylarge band gaps; thus, their absorption and dispersion can generally be neglected over the rangeof wavelengths considered in this work [26]. Errors can also arise due to discretization, whichcan be reduced at higher resolutions. Apart from these approximations, both of our calcula-tion methods for the optical properties are exact. Our two methods agree well when applied tosample 1D and 2D problems, even in the presence of dispersion.The emissivity of each structure can be calculated from the absorptivity computed above viaKirchhoff’s law of thermal radiation, which states that the two quantities must be equal at everywavelength for a body in thermal equilibrium [27].The ﬁgure of merit, as deﬁned below for each physical system, must be optimized overall optimization parameters. This global optimum is found through the application of themulti-level single-linkage (MLSL), derivative-based algorithm using a low-discrepancy se-quence (LDS) [28]. This algorithm executes a quasi-random (LDS) sequence of local searchesusing constrained optimization by linear approximation (COBYLA) [29], with a clusteringheuristic to avoid multiple local searches for the same local minimum. We veriﬁed that otherglobal search algorithms, such as DIRECT-L [30], yield similar results. This ability to di-rectly utilize and compare multiple optimization packages on the same problem is providedby the NLopt package, written by the present authors and freely available on our website,
http://ab-initio.mit.edu/nlopt
.

Search

Similar documents

Tags

Related Search

Global Optimization of Mining ComplexesModernism in Design and the Idea of ForeordaiDesign and thermal modeling of radially confiDesign and Technological Planning of ArchitecDesign and Stress Analysis of Structures UsinIndigenous and Global Aspects of PsychologicaDesign and Optimization of low-power \u0026 Design of High Speed and Low Power ComparatorRobust Design and Design of OptimizationDesign and development of high performance ma

We Need Your Support

Thank you for visiting our website and your interest in our free products and services. We are nonprofit website to share and download documents. To the running of this website, we need your help to support us.

Thanks to everyone for your continued support.

No, Thanks